70 5. Macroscopic measurements in Cr7Ni and Cr8Ni
Figure 28: This figure reports one of the degenerate configurations corresponding to an S = 0 ground state calculated for the classical version of the model of Cr8Ni. The blue cone represents the Nickel ion. Within this reference frame, the angle between spin 4, 5 (whose bond is opposite to the Nickel site) and the spin of the Ni ion along z is
≈78◦, while the angle between spin 4 and 5 is ≈156◦, being z the axis perpendicular to the plane of the ring. Therefore the knot is delocalized in the eight Cr ions with the sites 4 and 5 having the same z component. The classic picture of the ground state holds most of the main features of the quantum S = 0 ground state obtained from exact diagonalization of the isotropic Heisenberg term in Eq. (80).
above-mentioned locking of the three spins in an S = 2 state. The meaning of the remaining < SN i· Si > correlations can be understood by inspecting the vector struc-ture of the classical ground state (see Fig. 28), which shows a pattern of correlations similar to that of the quantum ground state: classically, the spins are oriented in a noncollinear fashion due to spin frustration. For instance, the Cr spins at sites 4 and 5 are almost lying in a plane perpendicular to the Ni spin which corresponds to nearly vanishing correlations < SN i · S4 > and < SN i · S5 > as shown in Fig. 27(b). On the other hand, quantum mechanically, the S=0 ground state approximately resonates among the infinite classical configurations. Hence, local magnetic moments vanish at low temperature due to quantum fluctuations, which is directly revealed by present NMR measurements.
5.3. Conclusions 71
Figure 29: (a) Schematic structure of the Cr8Ni cluster with the enumeration of bonds and spin sites. (b) Scalar products Strimer· Si show how frustration is distributed in magnetic sites from 1 to 7, being Strimer = S18+ S9. (c) Scalar product SN i· Si. Assuming the Nickel spin in position 9 to be aligned along z-axis, SN i· Si reflects the non uniform distribution of local moments in the ground S = 0 state. (d) Excitation energy of the first excited state S = 1 with respect to the ground state S = 0 as a function of the exchange bonds. It is straightforward to note that bonds 1 and 9 do not cooperate to the first excitation. This occurs since JCr−N i >> JCr−Cr and thus the trimer is blocked in a Strimer= 1 state.
72 5. Macroscopic measurements in Cr7Ni and Cr8Ni
at very high fields. In particular, in Cr7Ni these results confirm that the microscopic picture derived from INS experiments [30,68] at zero field perfectly holds even for spin multiplets not accessible to the INS tecnique. Besides, in Cr8Ni high field magneti-zation together with specific heat measurements at low temperatures( below 1K) give clear evidence for a spin singlet ground state at zero magnetic field in agreement with theoretical calculations based on an Hamiltonian including Heisenberg, crystal field and Dzyaloshinski-Moriya interactions. In particular, the field-dependence of the specific heat and the widths of the magnetization steps provide strong evidence of the presence of level anticrossings due to antisymmetric terms in the Hamiltonian. The proton NMR measurements confirm the above results indicating that the local spin density is zero in the ground state as a result of quantum fluctuations among frustrated local spins configurations .
Relaxation dynamics in magnetic molecules
In the present chapter the theory of relaxation of molecular observables developed in the following section and derived in Ref.  will be applied to several types of magnetic molecules. The Mn12, Fe8 nanomagnets, the Fe30 icosidodecaedron, the V12 antiferro-magnetic cluster containing ions with spin 1/2 and the Cr7Ni heterometallic ring will be taken into account and investigated as regards their spin dynamics. Irrespective of the different topology, local ions and microscopic interactions, all studied molecules show similar relaxation mechanisms. In many cases we will show how the NMR technique can provide useful information about the relaxation dynamics in magnetic molecules.
6.1 Decoherence and relaxation phenomena in mag-netic molecules
The interaction of electronic spins with other degrees of freedom such as phonons causes decoherence in the time evolution of molecular observables, thus leading to relaxation dynamics. This is reflected in the irreversible evolution of the density matrix ρst(t), evaluated in the basis of exact eigenstates of the cluster Hamiltonian [H|si| = Es|si].
Since we are interested in relaxation phenomena characterized by time scales much longer than the free evolution periods of the system 2π~/(Es−Et), the evolution of the diagonal matrix element ρss(t) = ps(t) can be decoupled from that of the off-diagonal ones ρs6=t(t) [secular approximation]. This allows a clear separation of quasi-elastic (QE) and inelastic (IE) spectral contributions in frequency domain. The former can
74 6. Relaxation dynamics in magnetic molecules
be detected by low-frequency experimental techniques such as AC suceptibility and NMR, while the latter are determined by the lifetimes of the involved pair of levels and can be probed by means of higher frequency techniques such as INS and electron spin resonance (or ESR).
Exploiting the so called secular approximation, the populations of the molecular eigen-states evolve, pt(t) through the well known rate master equations
where Wst, the st element of the rate matrix W, represents the probability per unit time that a transition involving |si and |ti levels occurs because of the interaction of the system with the heat bath (Wss = − PtWts). In the range of temperatures of our interest, dechoerence and relaxation phenomena are caused by the interaction of electronic spins with phonons. In magnetic molecules with local spin s > 1/2 the main contributions to this coupling come from modulation of the local rank-2 crystal fields (CFs)P
qb(i)q2Oq2(si), with Oq2(si) Stevens operator equivalents for spin i and bq2(i) CF parameters. This leads to the following spin-phonon coupling potential:
V = X
CQ(i, k, σ), T2Q(si)(ckσ + c+−kσ), (85)
where N is the number of ions in the cluster, CQ(i, k, σ) is the coupling constant between the Q-type electric quadrupole on ion i and the phonon modes of wave vector k and branch σ. Adopting a Debye model for phonons and choosing coupling coefficients CQ(l, k) independent of l and Q we obtain the following transition rates Wst between levels s and t (in first order perturbation theory):
Wst = γπ
with n(x) = (eβ~x− 1)−1, ∆st = (Es− Et)/~. In this simple model, γ is the unique free parameter: it represents the spin-phonon coupling strength. Another possible choice for the magnetoelastic coupling leads to the following expression:
Wmn = γπ2∆3mnn(∆mn) X
× hn| Oq1,q2(sj)|mi , (87) where Oq1,q2(si) = (sq1,isq2,i+ sq2,isq1,i)/2 are quadrupolar operators which give rise to a spherically symmetric magnetoelastic (ME) coupling for the transition metal ions in
6.1. Decoherence and relaxation phenomena in magnetic molecules 75
a cluster with s > 1/2 and q1, q2 = x, y, z . In Section 6.4 we will investigate the relaxation dynamics in a molecule containing s = 1/2 ions. In this case, we recall that phonons are assumed to cause the modulation of next neighbours anisotropic exchange, since there are no local crystal field terms for ions with spin 1/2.
In order to understand the mechanisms which governs the spin dynamics in magnetic molecules, the Fourier transform SA,B(ω) of the cross correlation functionh∆A(t)∆B(0)i, where A and B are two generic molecular observables, has to be evaluated. First of all, the fluctuation dissipation theorem allows to relate the imaginary part of the gen-eralized susceptibility χ00A,B(ω), the real part of the Laplace transform ˜R0A,B(z) of the relaxation function RA,B(t) and the SA,B(ω) together:
SA,B(ω) = 2kBT χ00A,B(ω)
ω = 2kBT ˜R0A,B(ω) (88)
The relaxation function is defined as lim→0(hA(t)i−hAieq)/, with a small perturbation
B switched off at t = 0. Acting inside the well established framework developed in [76,77], we are able to calculate the RA,B(t) by first-order perturbation theory. Being H0 the unperturbed Hamiltonian of our spin system and |ni and En(0) its eigenvectors and eigenvalues respectively, at t < 0 we introduce the small perturbation B (e.g. a small magnetic field which couples with the observable B). As a result, retaining only first-order terms in B, at t = 0 the density matrix reads as follows:
ρ(t = 0) = X
Z |˜ni h˜n|
p(eq)n |ni hn| + p(eq)n β(Bnn− hBi) |ni hn| −
En(0)− Eq(0)|qi hn| + Bnq
En(0)− Eq(0) |ni hq|
(89) where |˜ni and En˜ are respectively the eigenvectors and eigenvalues of the complete Hamiltonian, p(eq)n = e−βEn(0)/Z0 is the nth diagonal density matrix element at equilib-rium, being Z0 the partition function of the unperturbed spin system. According to the theory presented in  for the irreversible evolution of the density matrix, the QE and IE part of ρ(t) at times t > 0 can be determined separately:
ρnn(t) = X
νnm(t)ρ(t = 0)mm (90)
ρmn(t) = Γnm(t)ρmn(t = 0) (91)
ν(t) = eW t (92)
76 6. Relaxation dynamics in magnetic molecules
is the propagator which gives the time evolution of the QE part of the density matrix, while
Γnm(t) = ei∆nmte−t/τnm (93)
is the IE propagator of ρ. Here τnm =−12(Γmm+ Γnn) is the average of the the lifetimes of levels n and m, and represents the time after which the phase coherence is lost .
Since we are interested in the QE part of spin dynamics, we calculate the evolutions of molecular observables neglecting the off-diagonal terms of the density matrix. As a result, we obtain:
RA,B(t) = lim→0hA(t)i − hAieq
p(eq)m Bmm− hBieq
Finally, we have to take the real part ˜R0A,B(iω) of the Laplace transform of RA,B(t):
R˜0A,B(iω) = βX
p(eq)m Bmm− hBieq ×
If we consider Eqs. (88) and (95) it should be noted that the QE part of the Fourier transform of the cross correlation function SA,B(ω) involves only the diagonal elements of observables A, B [20,21]. Thus, the Fourier transform for the QE part of a general spin-spin correlation functions is:
SA,B(ω) = X
× (Aqq− hAieq)Re (
where p(eq)t is the equilibrium population of the t-th level, Btt =ht|B|ti and W is the so-called rate matrix. Furthermore, since we are mainly interested in the dynamics of magnetization we take A = B = Sz and write Eq. (96) as:
SSz,Sz(ω, T, B) = X
A(λi, T, B) λi(T, B)
λi(T, B)2+ ω2 (97)
where λi(T, B) = 1/τQE(i) are the eigenvalues of −W. As a consequence, the autocorre-lation of magnetization is given by a sum of lorentzians centered at zero frequency and
6.1. Decoherence and relaxation phenomena in magnetic molecules 77
with width λi(T, B), and decays as a sum of exponentials with characteristic times τQE(i). Here the A(λi, T, B) coefficients represent the weights of the N possible lorentzians, N being the dimension of the Hilbert spin space of the molecule. Each τQE(i) refers to a particular spin-bath relaxation channel, given by the corresponding eigenstate |wii of W: the composition of|wii in terms of the molecular eigenstates gives the complete re-laxation path. Further information on the spin-bath dissipation channels is contained in the N level lifetimes τlif e(i) defined as τlif e(i) = [−Wii]−1 = [P
jWj←i]−1: this is the inverse of the sum of all transition rates between the considered i level and all other ones according to the selection rules imposed by spin-bath interaction. The two sets of τQE(i) and τlif e(i) times contain complementary information on the QE part of relaxation dynamics.
The electronic dynamic properties of magnetic molecules can be probed by NMR. In fact, the measured longitudinal relaxation rate 1/T1 is given by a linear combination of local spin correlation functions through the Moriya formula :
T1 = X
Ssqi,sq0j (−ωL) + S
where N is the number of magnetic ions in the cluster, αqqij0 are the geometric coefficients which depend on the positions of ions i and j and the probed nuclei, while Ssq
i,sq0j (ωL) is the Fourier transform of the cross correlation function calculated at the Larmor frequency of hydrogen nucleus ωL = γB, being γ the proton gyromagnetic ratio and B a magnetic field applied along z [see Eq. (97)]. Since far from level crossings ωL << ∆mn= ~/(Em− En), with Em, En eigenvalues of the cluster Hamiltonian, only the QE part of Ssq
i,sq0j (ωL) contributes to 1/T1, i.e. that calculated by means of Eq.
(96). Furthermore, as long as anisotropy can be neglected, ht|sx(i)|ti = ht|sy(i)|ti = 0 since from Eq. (96) it follows that only α = β = z terms are non zero. In addition for a magnetic ring ht|sz(i)|ti = ht|sz(j)|ti = 1/Nht|Sz|ti where Sz is the z component of the total spin operator S. Thus Eq. (98) reduces to:
= GSSz,Sz(ωL), (99)
where G is a geometric scale factor which accounts for the positions of hydrogens probed by NMR. This results holds also in the case of nanomagnets with easy-axis anisotropy, provided that the magnetic field is applied along the easy-axis direction. As a consequence the NMR techinque constitutes a probe of the dynamics of magnetization in most of magnetic molecules . The results we will see in this chapter well reproduce
78 6. Relaxation dynamics in magnetic molecules
0 . 1 0 . 2 0 . 3 0 . 4 0 . 5 0 . 6 - 1 6
- 1 4 - 1 2 - 1 0 - 8 - 6 - 4 - 2
1 / T ( 1 / K )
3 . 0 E - 3 6 . 2 E - 3 1 . 3 E - 2 2 . 6 E - 2 5 . 5 E - 2 1 . 1 E - 1 2 . 3 E - 1 4 . 8 E - 1 1 . 0 E 0
Figure 30: Calculated frequency weights A(λ, T, B) of the magnetization autocor-relation function vs 1/T . The y axis represents Log10(λ). The color maps Log10[A(λ, T, B)/(χT )]. The spectrum have been normalized by χT , since χT de-termines the size of equilibrium fluctuations. The red line in the spectrum represents the dominant frequency in the spectrum and follows the Arrhenius law. The parameters for Mn12spin Hamiltonian were derived by inelastic neutron scattering experiments .
the experimental curves and indicate that the T -dependence of NMR 1/T1 may or may not show any sharp peak. This can be understood noting that in agreement with previous studied molecules [11,10,20] the frequency spectrum of a given molecule at low T is dominated by a single lorentzian of characteristic frequency λ0. In fact, as long as there is a λ0 with appreciable weight, from Eq. (97) it can be argued that only when λ0 = ωL 1/T1(T ) should peak. Therefore, the NMR technique can probe the characteristic times of the spin dynamics in magnetic molecules.